Crystal Structures, Electronic Structures, and Physical Properties of Tl4MQ4 (M = Zr or Hf; Q = S or Se)
Cheriyedath Raj Sankar; Savitree Bangarigadu-Sanasy; Abdeljalil Assoud; Holger Kleinke; Inorganic Chemistry 50 (2011) 245–249; doi:10.1021/ic101925a

data_4324131
_publ_section_title
;
 Crystal Structures, Electronic Structures, and Physical Properties of
 Tl4MQ4 (M = Zr or Hf; Q = S or Se)
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              245
_journal_page_last               249
_journal_paper_doi               10.1021/ic101925a
_journal_volume                  50
_journal_year                    2011
_chemical_formula_sum            'S4 Tl4 Zr'
_chemical_formula_weight         1036.94
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                103.8710(10)
_cell_angle_beta                 105.0280(10)
_cell_angle_gamma                90.1380(10)
_cell_formula_units_Z            5
_cell_length_a                   9.0370(5)
_cell_length_b                   9.0375(5)
_cell_length_c                   15.4946(9)
_cell_measurement_temperature    296(2)
_cell_volume                     1183.73(12)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.993
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0560
_diffrn_reflns_av_sigmaI/netI    0.0711
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            16813
_diffrn_reflns_theta_full        30.00
_diffrn_reflns_theta_max         30.00
_diffrn_reflns_theta_min         3.00
_exptl_absorpt_coefficient_mu    69.694
_exptl_absorpt_correction_T_max  0.3362
_exptl_absorpt_correction_T_min  0.0438
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   'APEX II'
_exptl_crystal_colour            dark-red
_exptl_crystal_density_diffrn    7.273
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             2140
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.02
_refine_diff_density_max         3.303
_refine_diff_density_min         -4.413
_refine_diff_density_rms         0.642
_refine_ls_extinction_coef       0.00099(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.054
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     206
_refine_ls_number_reflns         6867
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.054
_refine_ls_R_factor_all          0.0567
_refine_ls_R_factor_gt           0.0422
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0002P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0892
_refine_ls_wR_factor_ref         0.0986
_reflns_number_gt                5377
_reflns_number_total             6867
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic101925a_si_001.cif
_cod_data_source_block           Tl4ZrS4
_cod_database_code               4324131